Abstract
Considerable attention is today devoted to the engineering of films widely used in photocatalytic, solar energy converters, photochemical and photoelectrochemical cells, dyesensitized solar cells (DSSCs), to optimize electronic time response following photogeneration. However, the precise nature of transport processes in these systems has remained unresolved. To investigate such aspects of carrier dynamics, we have suggested a model for the calculation of correlation functions, expressed as the Fourier transform of the frequencydependent complex conductivity σ(ω). Results are presented for the velocity correlation functions, the mean square deviation of position and the diffusion coefficient in systems, like TiO_{2} and doped Si, of large interest in present devices. Fast diffusion occurs in short time intervals of the order of few collision times. Consequences for efficiency of this fast response are discussed in relation to nanostructured devices.
Keywords:
Correlation Functions; Diffusion; FrequencyDependent Complex Conductivity; Nanostructures; Semiconducting Oxides; Montecarlo SimulationNano Express
One of the most important aspects of nanostructures concerns charge transport, which can be influenced by particle dimensions and assume different characteristics with respect to those of bulk. In particular, if the mean free path of charges due to scattering phenomena is larger than the particle dimensions, one has a mesoscopic system, in which the transport depends on dimensions and one might correct the transport bulk theories by considering this phenomenon. These problems occur also in a thin film, in which the smallest dimension can be less than the free displacement and therefore require variations to existing theoretical transport bulk models. This situation occurs particularly in connection with metal oxide, like transparency, hardness, etc. Therefore a rigorous knowledge of transport properties is to be acquired. To establish the applicability limit of a bulk model and to investigate the time response of systems at nanoscale we have performed a new approach based on correlation functions obtained by a Fourier transform of the frequencydependent complex conductivity of the system [1]. With this method it is possible to calculate these functions using experimental data obtained by various films, like TiO_{2} and ZnO also in the form of nanowires, which have increasing interest for their technological, chemical and biomedical applications and which are engineered to reach the desired technical features. Also, the mesoporous films play a very important role, for their applications in devices for energy generation, photocatalytic processes in environment remediations and for the useful electronic propertiestechniques, in particular the Timeresolved THz spectroscopy (TRTS) [2,3]. Starting from the Drude–Lorentz model [4,5] we have obtained directly the correlation function of velocities, the quadratic average distance crossed by the charges as a function of time and the diffusion coefficient D.
From a mathematical viewpoint, the Kubo relation of the linear response must be inverted. But, due to the presence of a half Fouriertransform, it is necessary to modify this relation in such a way that the whole time axis (∞, +∞) occurs. This procedure is not trivial and not previously found in the literature.
This new formula can be obtained by relying on linear response theory; we have started considering a system with an hamiltonian of the form:
with H_{1} having small effects respect to H_{0}, and negligible in the remote past (adiabatic representation). In the case of an electric field of frequency ω we have:
For an electric field constant in space and depending on time as:
the time dependent corresponding current is:
Following the standard timedependent approach [4], we derived a general formula for the linear response of a dipole moment density
From Eq. 5 we have deduced the real part of σ(ω), denoted in the form σ'(ω) as:
where S_{βα}(ω)is the quantity:
The quantity 〈···〉_{T} is the thermal average, and the exponential factor arises from equilibrium thermal
weights for Fermi particles. By considering the identity
The integral in Eq. 8 spans the entire t axis, so we can perform the complete inverse Fourier transform of this equation. It gives:
with V the volume of the system, K the Boltzmann's constant, T the temperature and σ'(ω) the real part of σ(ω), given by:
where n is the carrier density, ω_{0} the proper oscillator frequency, 1/τ the collision frequency [4,5].
The mean squared displacement in relation with the correlation function of velocities is given by:
By integration of Eq. 9 with Eq. 10, we deduced all the results for
The main advantage of this new formulation is the disposal of exact results for describing
the dynamic behaviour, as extracted by timeresolved techniques. In our analytical
procedure we have distinguished the case ω_{o} = 0 from the case ω_{o} ≠ 0. For this latter, three cases occur in connection with the sign of the quantity
We have used our results for discussing transport in a conventional semiconductor such as doped Si, non conventional TiO_{2} and other systems where anomalous transport has been found.
The most important characteristics of the results are illustrated by concrete examples in Figures 1, 2, 3, 4, and 5.
Figure 1. R^{2} vs. x = t/τ for some representative values of τ, typical of doped Si [7](ω_{0} = 0, T = 300 K) (Drude model). A complete description of R^{2} for Si requires the evaluation of the contribution of the Drude–Lorentz part (see text).
Figure 2. R^{2} vs. x = t/τ for 2 values of τ (ω_{0} = 1.12 × 10^{11}Hz dotdashed; ω_{0} = 2.24 × 10^{11}Hz dashed) for TiO_{2} (m = 6m_{e}, T = 300 K). Saturation values occur at sufficiently large t.
Figure 3. R^{2} vs. x = t/τ at constant ω_{0}τ, for 3 values of τ (ω_{0} = 0.5 × 10^{13}Hz solid; ω_{0} = 10^{13}Hz dotdashed; ω_{0} = 0.5 × 10^{14}Hz dashed) for TiO_{2} (m = 6m_{e}, T = 300 K).
Figure 4. Velocity correlation function vs. x = t/τ for two values of α_{R} (
Figure 5. Velocity correlation function vs. x = t/τ for some values of α_{I} (
In Figure 1, we show R^{2} for doped Si. For this semiconductor, the conductivity is the contribution of two terms, a Drude–Lorentz term and a Drude term [7]. At large times the Drude–Lorentz term leads to an R^{2} approaching a constant value (see Figure 2), while the Drude term alone (Figure 1) is the dominant term at large times. Therefore for sufficiently large times, only the Drude term survives.
We observe that the linear relation at large times becomes quadratic at smaller times. The crossover between the two regimes occurs at times comparable to the scattering time. This means that diffusion occurs after sufficient time has elapsed so that scattering events become significant, while at smaller times the motion is essentially ballistic.
In Figures 2 and 3R^{2} saturates at high t. The plateau value may assume high values so that R may be larger than the size of the nanoparticles composing the films. In general, these features indicate quite enhanced mobility of carriers in the nanoporous films at small times, in contrast with a commonly expected low mobility in a disordered network.
From these figures we can evaluate the diffusion coefficient
From the other hand, much smaller D can develop at long times, with values D = 10^{4}–10^{6} cm^{2}/s typical of a disordered strong scattering system. So, our results indicate quite different behaviour in Si where normal diffusion occurs, and in TiO_{2} where the Drude–Lorentz model indicates anomalous diffusion.
The physical reason and mechanism of such increase can be traced back to ballisticlike motion of the carriers at early time when scattering is moderate yielding normal diffusion satisfying Eintein's rule and to strong localization due to the scattering at long times with anomalous diffusion with depression of D.
Figures 4 and 5 report the behaviour of the velocity correlation function.
We observe that, according to the equations of our model [8,9], the correlation function of velocities is never a single decreasing exponential of time, but it is in general a more complicated combination of exponentials, or an oscillating function of time.
When
When
The results above give a precise indication on response times of a system subjected to charge motion. In the case of doped Si [7] we have verified the Einstein rule, giving rise to normal diffusion. In the case of TiO_{2 }[2,3], anomalous diffusion is found with timedependent diffusion coefficient vanishing at long times and oscillating behaviour in time of the transport parameters. We have compared our effective diffusion coefficients directly with experimental results [1113] and with Monte Carlo simulations [14,15], which take into account the overall mechanisms of scattering, including phonons, imperfections and doping centres, and traps, finding that the diffusion coefficient reproduces the values of experimental or simulated coefficients.
We suggest the possibility that our results can give an explanation of the ultrashort times and of high mobilities with which the charges spread in mesoporous nanoparticle TiO_{2} systems, of deep interest in photocatalitic and photovoltaic systems [16,17]. In particular, the relative short times (few τ) with which charges can reach much larger distances than typical dimensions of nanoparticles indicate easy diffusion for charges photoproduced inside the nanoparticles towards the surface. The unexplained fact found experimentally of ultrashort injection of charge carriers (particularly in Graetzel's cells) can be related to this phenomenon [16,17].
Similar high diffusivity is found in a number of other devices, i.e. GaAs nanowires and ZnO nanoparticles on which terahertz timeresolved spectroscopy has revealed different time transport regimes with high diffusion processes at short times of the order of the scattering time and longer time localized motion due to the effects of scattering [18,19]. Interpretations of these results in terms of the model suggested here can be given.
Recently, an approach for converting nanoscale mechanical energy into electrical energy has been suggested by using piezoelectric zinc oxide (ZnO) nanowires and TiO_{2 }[20]. Such devices have been shown to convert mechanical energy into electric energy with typical ∼1 nW output power per cm^{2} area. These unexpected efficiencies can be explained by anomalous high diffusion in the oxides of the type presented here.
In summary, we have evaluated the correlation functions for systems for which the
Drude–Lorentz model is valid through the formulation of a new Drude–Lorentzlike model
[8,9], in which such functions can be obtained as complete Fourier transform of the real
part of the frequencydependent complex conductivity σ(ω). From our results we deduce some important consequences connected with the nanometric
film systems, in particular the possibility of a fast response of the transport of
charge carriers with a direct consequence for the efficiencies of present devices
based on such systems. Of particular interest for nanostructures is the fact that
the limiting value of
References

Ventura PJ, Costa LC, Carmo MC, Roman HE, Pavesi L:
J Porous Mater. 2000, 7:107. Publisher Full Text

Hendry E, Wang F, Shan J, Heinz TF, Bonn M:
Phys Rev B. 2004, 69:081101(R). Publisher Full Text

Ziman M: Principles of the Theory of Solids. Cambridge University Press, New York; 1979.

Kittel C: Introduction to Solid State Physics. Wiley, New York; 1995.

Rudin W: Real and Complex Analysis. McGrawHill International Editions: Mathematics Series, McGrawHill Publishing Co.; 1987.

Phys Rev A. 2008, 77:013811. Publisher Full Text

J Comput Theor Nanosci. 2011, 8:1. Publisher Full Text

Di Sia P, Dallacasa V, Dallacasa F:
J Nano Res. 2010, 11:45. Publisher Full Text

Phys Rev B. 2001, 64:155106. Publisher Full Text

Phys Rev B. 2000, 61:4699. Publisher Full Text

Kambili A, Walker AB, Qiu FL, Fisher AC, Savin AD, Peter LM:
Physica E Low Dimens Syst Nanostruct. 2002, 14:203. Publisher Full Text

J Phys Chem B. 1999, 103:782. Publisher Full Text

J Phys Condens Matter. 1990, 2:4717. Publisher Full Text

Bettinelli M, Speghini A, Falcomer D, Daldosso M, Dallacasa V, Romanò L:
J Phys Condens Matter. 2006, 18:S2149. Publisher Full Text

Inorg Chem. 2005, 44(20):6841. PubMed Abstract  Publisher Full Text

J Photochem Photobiol C: Photochem Rev. 2003, 4:145. Publisher Full Text

Dallacasa V, Dallacasa F, Di Sia P, Scavetta E, Tonelli D:
J Nanosci Nanotechnol. 2010, 10:1043. PubMed Abstract  Publisher Full Text

Parkinson P, LloydHughes J, Gao Q, Tan HH, Jagadish C, Johnston MB, Herz LM:
Nano Lett. 2007, 7(7):2162. Publisher Full Text

Adv Funct Mater. 2008, 18:3553. Publisher Full Text